Indian Standard ’ RnfBimcd lw7 ’
-CONCRETE MASONRY UNITS
PART I HOLLOW AND SOLID CONCRETE BLOCKS
( Second Revision)
Third Reprint OCTOBER 1990
0 Copyright 1980
BUREAU OF INDIAN STANDARDS
MANAK BHAVAN. 9 BAHADUR SHAH ZAFAR MARG
Or6 April 1980
( Reaffirmed 1998 )
IS : 2185( Part I ) - 1979
CONCRETE MASONRY UNITS
PART I tlOLLOW AND SOLID CONCRETE BLOCKS
( Second Revision)
Cement and Concrete Sectional Committee, BDC 2
Ds H. C. VISVESVARAYA Cement Research Institute of India, New Delhi
STANDARDS( B & S )
Research, Designs & Standards Organization
( Ministry of Railway6 )
&ro? 6~~s ( B & S ) ( Ahnate )
SBRI K. C AQ~ARWAL Hindustan Prefab Ltd, New Delhi
SEX1C. L. KASLIW~L( Altctaati)
SHRIK. P. ~&.NEBJEE Lanen & Toubro Ltd, Bombay
SARI HARISHN. MALANI( Alternate )
SHRIR. N. BANSAL
SHRI T. Cl.GARU( Altanate j
BeasDesigns Organization, Nangal Township
DR N. S. B~AL Struct~t;~e~gineering Research Centre ( CSIR ),
SHRIR. V. CHALAPATHIRAO Geological Survey of India, Calcutta
SHBIS. ROY ( Alternate )
Central Public Work6 Department, New Delhi
( DESIQNS) III ( Aftaat6)
CHIEFENQINEER( PROJECTS )
DIsaaToR, IPRI ( Ahcrnat6 )
Irrigation Department, Government of Punjab
DIRECTOR( CSMRS ) Central Water Commission, New Delhi
DEPUTY DIRECTOR( CSMRS)
( Akrnat6 )
SHRIAMITABHAGHOSH National Test House, Calcutta
SHRI E.K. &MACIHANDRAN
( dhrnuts )
( Continurd on /hl#6 2 )
Q copyrqht 1980
BUREAU OF INDIAN STANDARDS
This publication is protected under the Znllian Co~vri& Act ( XIV of 1957) and
reproduction in whole or in part by any means except with written permission of the
publisher shall be deemed to be an infringement of copy1ight under the said Act.
(Continuedfrom pags 1)
DR R. K. GHOSH
Central Road Research Institute ( CSIR ),
SHXI Y. R. PHULL ( Alternatc I )
SHRI M. DINAKARAN ( Alternate II)
Ds R K. GHOSH Indian Roads Congress, New Delhi
SRRI B. R. GOVIND Engineer-in-Chief’s Branch, Army Headquarters
SHRIP. C. JAIN ( Altamate )
SXRI A. K. GUPTA HydeHabard,b:;bestos Cement Products Ltd,
DR R. R. HATTIAN~ADI The ‘Associated Cement Companies Ltd,
SHRI P. J, JAOUS ( Altematu )
DR IQBAL ALI Engineering Research Laboratories, Hyderabad
SH~I M. T. KANSE Directorate General of Supplies & Disposals,
SHRI S. R. KULKARNI M. N. Dastur & Co ( Pvt ) Ltd, Calcutta
SHRI S. K. LAHA The Institution of Engineers ( India ), Calcutta
SHRI B T. UNW~LLA ( Alternate )
DR MOWAN RAI
Dn.S. S. REHSI ( Alternate )
Centffajoryezding Research institute ( CSIR ),
SHRIK. K. NAMBIAR In Personal Capacity ( ‘Ramanalqya’ II. First
Crescent Park Road, Gandhinagar, Adyar,
DR A. V. R. RAO National Buildings Organization, New Delhi
SHRIK. S. SRINIVASAN ( Altematr )
SHRI T. N. S. RAO Gammon India Ltd, Bombay
SHRI S. R. PINHEIRO ( Alternate )
SERI ARJ~N RIJHSINQHANI Clement Corporation of India Ltd, New Delhi
SHRI K. VITHAL RAO ( Alternate )
SEO~ETARY Cent;lw tTh;d of irrigation and Power,
DEPUTY SECRETARY ( I ) ( Alrsrnatr )
SERI N. SEN Roads Wing ( Ministry of Shipping and
SRRI J. R. K. PRA~AD ( Altanatr )
SERI K. A. SUBRA~ANIAM The India Cements Ltd, Madras
SHBI P. S. RAMACHANDRAN f Altmnats j
SUPESINTENDZN~ ENIXN~~ER ’ Public- Works Department, Government of
( DESIGNS ) Tamil Nadu, Madras
EXECUTIVE ENQINEER( SM&R
DIF-ISION) ( Altarnatc 1
SHRI L. SWARO~P‘ Dalmia Cement ( Bharat ) Ltd, New Delhi
&RI A. V. RAMANA ( Alternate )
SHRI B. T UNWALLA The Concrete Association of India, Bombay
SHRI T. M. MENON ( Alternate )
SHRI D. AJITHA SIMHA, Director General, BIS ( Ex-oJcioMember ) _
Director ( Civ Engg )
SHRI M. N. NEELAK~DE~
Assistant Director ( Civ Engg ), BlS
( Continurd on &age 24 )
CONCRETE MASONRY UNITS
PARTI HOLLOW AND SOLID CONCRETE BLOCKS
( Second Revision)
0.1 This Indian Standard ( Part I ) ( Second Revision ) was adopted by
the Indian Standards Institution on 25 November 1979, after the draft
finalized by the Cement and Concrete Sectional Committee had been
approved by the Civil Engineering Division Council.
0.2 This standard .was first published in 1962 and subsequently revised in
1967. The second revision is being published under the modified title
‘Specification for concrete masonry units : Part I Hollow and solid
concrete blocks’. It is proposed to bring out Part II and Part III
subseq:,c rtly; Part 11 covering lightweight concrete masonry units
( revision of IS : 3590-1966* ) and Part III covering aerated concrete
masonry units ( revision of IS : 5482-1969t ).
0.2.1 This standard incorporates significant modifications especially
with regard to the classification of the blocks and physical requirements
such as dimensions, compressive strength values, water absorption and
drying shrinkage. Also in this version, apart from covering hollow blocks
of open cavity type, hollow blocks of closed cavity type-have-been covered.
Another distinct feature in this revision is that concrete masonry units of
load bearing and non-load bearing category have been separately treated
to the extent possible.
0.3 Concrete masonry, already extensively used in building construction
abroad, is likely to make very considerable headway in this country
because of the many advantages, such as durability, strength and struc-
tural stability, fire resistance, insulation, and sound absorption it possesses..
Concrete masonry constructron is also economical because of the following
a) The units are relatively large and true in size and shape. This /
insures rapid construction so that more wall is laid per man-hour
than in other types of wall canstruction;
*Specification for load bearing lightweight concrete blocks.
$Specification for autoclaved cellular concrete blocks.
IS : 2185 ( Part I ) - 1979
b) -Fewer joints result in considerable saving in mortar as compared
to normal masonry construction, and also in increasing the
strength of the wall; and
c) The true plane surfaces obtained obviate necessity of plaster for
unimportant buildings situated in low rainfall areas; even when
plaster is used for any reason, the quantity required for satisfac-
tory coverage is significantly small.
0.3.1 Concrete masonry has an attractive appearance and is readily
adaptable to any style of architecture. It lends itself to a wide variety of
surface finishes for both exterior and interior walls. It may also be
finished with cement plaster, gauged withlime or a plasticizer. Concrete
masonry units provide a strong mechanical key, uniting the concrete
masonry backing and the plaster finish in a strong permanent bond.
0.4 Concrete masonry units are used for both load-bearing and non-load
bearing walls, for partitions and panel walls, as backing for other types
of facing material, for piers, pilasters and columns, for retaining walls,
garden walls, chimneys and fire places, as fillers in concrete joist floor
construction, and as shuttering for beams, columns and lintels.
0.5 The hollow ( open and closed cavity ) and solid concrete masonry
units covered by this standard are made with normal weight aggregates
and are known as normal weight units. The hollow load-bearing concrete
block of the standard 400 X 200 x 200 mm size will weigh between 17
and 26 kg when made with normal weight aggregate. Normal weight
units are made with such aggregates as sand, gravel, crushed stones and
0.6 For the purpose of deciding whether a particular requirement of
this standard is complied with, the final value, observed or calculated,
expressing the result of a test, shall be rounded off in accordance with
IS : 2-1960*. The number of ‘significant places retained in the rounded off
value should be the same as that of the specified value in this standard.
1.1 This standard ( Part I ) covers the following concrete masonry
building units which are used in the construction of load-bearing and
a) Hollow ( open and closed cavity ) load bearing concrete blocks,
b) Hollow ( open and closed cavity ) non-load bearing concrete
c) Solid load-bearing concrete blocks.
*Ruler for roundingoff numerical values( rc~isrd).
2.0 For the purpose of this standard, the following definitions shall apply.
2.1 Block - A concrete masonry unit, either hollow ( open or closed
cavity ), or solid ( other than units used for bonding, such as a half
block ), any one of the external dimension of which is greater than the
corresponding dimension of a brick as specified in IS : 3952-1978*, and
of such size and mass as to permit it to be handled by one man. Further-
more, to avoid confusion with slabs and panels, the height of the block
shall not exceed either its length or six times its width.
2.2 Block Dqnsity - The density calculated by dividing the mass of a
block by the overall volume, including holes or cavities and end recesses.
2.3 Drying Shrinkage - The difference between the length of specimen
which has been immersed in water and then subsequently dried “to cons-
tant length, all under specified conditions; expressed as a percentage of
the dry length of the specimen.
2.4 Face’ Shells - The two outer plates of the hollow concrete block.
These are connected together by webs. .“.I
2.5 Gross Area - The totalarea occupied by a block on its bedding
face, including areas of the cavities and end recesses.
2.6 Height - The vertical dimension of the exposed face of ~a block,
excluding any tongue or other device designed to provide mechanical
2.7 Hollow ( Open or Closed Cavity ) Block - A block having one
or more large holes or cavities which either pass through the block ( open
cavity ) or do not effectively pass through the block ( closed cavity ) and
having the solid material between 50 and 75 percent of the total volume
of the block calculated from the overall dimensions.
2.8 Length - The horizontal dimension of the exposed face of a block,
excluding any tongue or other device designed to provide mechanical
2.9 Moisture Movement - The difference between the length of the
specimen when dried to constant length and when subsequently immersed
in water, all under specified conditions, expressed as a percentage of the
dry length of the specimen.
*Specification for burnt clay hollow blocks for wallsand partitions (JFrsf r&ion ),
2.10 Solid Block - A block which has solid material not less than 75
percent of the total volume of the block calculated from the overall
2.11 Webs - The solid sections of the hollow concrete blocks which
connect the face shells.
2.12 Width - The external dimension of .a block at the bedding plane,
measured at right angles to the length and height of the block.
3. DIMENSIONS AND TOLERANCES
3.1 Concrete masonry building units shall be made in sizes and shapes to
fit different construction needs. They include stretcher, corner, double
corner or pier, jamb, ‘header; bull nose, and partition block, and concrete
3.2 Concrete Block - Concrete block, hollow ( open or ‘closed cavity )
or solid shall be referred to by its nominal dimensions. The term ‘nominal’
means that the dimension includes the thickness of the mortar joint.
Actual dimensions shall be 10 mm short of the nominal dimensions ( or
6 mm short in special cases where finer jointing is specified ).
3.2.1 The nominal dimensions of concrete block shall be as follows:
Length 400, 500 or 600 mm
Height 200 or 100 mm
Width 50, 75, 100, 150, 200, 250 or 300 mm
In addition, block shall be manufactured in half lengths of 200, 250
or 300 mm to~correspond to the full lengths.
The nominal dimensions of the units are so designed that taking
account of the thickness of mortar joints, they will produce wall lengths
and heights which will conform to the principles of modular CO-
3.2.2 Blocks of sizes other than those specified in 3.2.1 may also be used
by mutual agreement between the purchaser and the supplier. In the
case of special concrete masonry unit,s such as jallie or screen wall block
and ornamental block, the specified sizes may not necessarily apply.
3.2.3 The maximum variation in the length of the units shall not be
more than f 5 mm and maximum variation in height and width of unit,
not more than f 3 mm.
3.2.4 Face shells and webs shall increase in thickness from the bottom
to the top of the unit. Depending upon the core moulds used, the face
shells and webs shall be flared and tapered or straight tapered, the
former providing a wider surface for mortar. The thickness of the face
shell and web shall be not less than the values given in Table 1, as
TABLE 1 m FACE SIELL AND WBB THICKNESSES
All dimensions in millimetres.
100 or less
Over 100 to 150
Over 150 to 200
3.3 Subjekt to the tolerances specified in 3.2.3 and the provisions of 3.4
the faces of masonry units shall be flat and rectangular, opposite faces
shall be parallel, and ~a11arises shall be square. The bedding surfaces shall
be at right angles to the faces of the blocks.
3.4 Blocks with Special Faces - Blocks with special faces shall be
manufactured and supplied as agreed upon between the supplier and the
4.1 Hollow (Open and Closed Cavity ) Concrete Blocks - The
hollow ( open and closed cavity ) concrete blocks shall conform to the
following three grades:
Grade A - These are used as load bearing units and shall have a
minimum block density of 1 500 kg/ma. These shall be manu-
factured for minimum average compressive strengths of 3’5, 4.5,
5’5 and 7’0 N/mtAa respectively at 28 days ( see Table 2 ).
Graile B - These are also used as load bearing units and shall
have a block density less than 1 500 kg/m3, but not less than
1 000 kg/ms. These shall Abemanufactured for minimum average
compressive strengths OF 2’0, 3’0 and 5’0 N/mms respectively at
28 days ( SGGTable 2 ).
c) Grade C - These are used as non-load bearing units and shall
have a block density less than 1 500 kg/ms, but not less than
1 000 kg/m*. These shall be manufactured for minimum average
compressive strength of 1’5 N/mm’ at 28 days ( see Table ~2).
4.2 Solid. Concrete Blocks - Grade D - The solid concrete blocks
are used as load bearing units and shall have a block density not
less than 1 800 kg/ms. These shall be manufactured for minimum average
compressive strengths of 4’0 and 5’0 N/mm* respectively ( see Table 2 ).
5.1 Cement - Cement complying .with any of the following Indian
Standards may be used at the discretion of the manufacturer:
IS : 269-1976 Specification for ordinary and low heat Portland cement
( third revision )
IS : 455-1976 Specification for Portland slag cement ( third revision )
IS : 1489-1976 Specification for Portland pozzolana cement
( second revision )
IS : 6909-1973 Specification for supersulphated cement
IS : 8041-1978 Specification for rapid hardening Portland cement
IS : 8042-1978 Specification for white Portland cement
IS : 8043-1978 Specification for hydrophobic Portland cement
5.1.1 When cement conforming to IS : 269-1976* is used, replacement
of cement by fly ash conforming to 1% 3812 ( Part I )-1966t may be
permitted I.$ to a limit of 20 percent. However, it shall be ensured that
blending of fly ash with cement is as intimate as possible, to achieve
5.2 Aggregates 2 The aggregates used in the manufacture of blocks at
-the mixer or the mixing platform shall be clean and free from deleterious
matter and shall conform to the requirements of IS : 383-1970#.
5.2.1 The grading of the combined aggregates shall conform as near as
possible to the requirements indicated in IS : 383-1970$. It is recom-
mended that the fineness modulus of the combined aggregates shall be
between 3’6 and 4.
*Specification for ordinary and low heat Portland cement ( third nvisiort).
$3prcification for fly ash : Part I For use as pozzolana.
SSpecification for coarse and fine aggregates from natural sources for concrete
( second m&ion ).
5.2.2 Fly ash conforming to IS : 3812 ( Part III )-1966* may be used
for part replacement of fine aggregate up to a limit of 20 percent.
5.3 Water - The water used in the manufacture of concrete masonry
units shall be free from matter harmful to concrete or reinforcement, or
matter likely to cause efflorescence in the units and shall conform to the
requirements of IS : 456-1978t.
5.4 Additives or Admixtures - Additives or admixtures may be added
either as additives to the~cement during manufacture, or as admixtures to
the concrete mix. Additives or admixtures used in the manufacture of
concrete masonry units may be:
a) accelerating, water-reducing
conforming to IS : 9103-1979$,
and air-entraining admixtures
b) fly ash conforming to IS : 3812 ( Part II )-1966&
c) waterproofing agents conforming to IS : 2645-197511, and
d) colouring pigments.
Where no Indian Standards apply, the additives qr admixtures shall
be shown,by test or experience, to be not detrimental to the durability of
6.1.1 The concrete mix used for blocks shall not be richer than one
part by volume of cement to 6 parts by volume of combined aggregates
6.1.2 In case of hand-moulded block where compaction is done
inanually, concrete mix should be sufficiently donsistent to enable
demoulding immediately after casting. The consistency of the mix should
be such that it may cohere when compressed in the hand without free
water being visible. Too little water causes the mix to be friable, while
too much water causes difficulty in the immediate withdrawal of the
*Specification for fly ash: Part III For use as fine aggregate for mortar and conctere.
t&de of practice for plain and reinforced concrete ( tltird rsoision).
SSpecification for admixtures for concrete.
§Sprc’ification for fly ash: Part II For use as admixture for concrete.
/[Specification for integral cement waterproofing compounds ( Jirst rmision).
6.13 In case of machine-moulded blocks, the web markings on the
units as they come from the machine give a good indication as to whether
the proper consistency of concrete has been used. In addition to the
grading of the aggregate and the quantity of cement, the amount of water
required f8r mix will depend to an extent on the type of machine on
which blocks are produced. It is possible to judge the proper consistency
by squeezing a handful of concrete mixture. When traces of moisture
show on’ the outside of the squeezed mass it is usually considered to be
6.2.1 Concrete shall normally be mixed in a mechanical mixer.
220.127.116.11 Mixing shall be continued until there is a uniform distribution
of the materials, and the mass is uniform in colour and consistency.
6.2.t.2 When hand mixing is permitted by the engineer-in-charge, ir
shall be carried out on a water-tight platform and’care shall be faken to
ensure that mixing is continued until the mass is uniform in colour and
consistency. Ten percent extra cement may be added when hand-mixing
is resorted to.
6.3 Placing and Compaction
6.3.1 In the case of manual compaction, the mixture shall be placed
into the mould in layers of about 50 to 75 mm and each layer thoroughly
tamped with suitable tampers until the whole mould is filled up and
struck off level with a trowel.
6.3.2 In the case of mechanical compaction, the mould shall be filled
up to overflow, vibrated or mechanically tamped and struck off level.
-6.3.3 After demoulding the blocks shall be protected until they are
sufficiently hardened to permit handling without damage.
6,4.1 The blocks hardened in accordance with 6.3.3 shall then be cured
in a curing water tank or in a curing yard ( see Note ), and shall be kept
continuously moist for at least 14 days. When the blocks are cured in an
immersion tank, the water of the tank shall be changed at least every
NOTE - The curing yard is a paved yard subdivided by shallow drains in 4 to 5 m
square platforms which are provided with water fountains in the centre. The blocks
are stacked on the platforms around the fountains, which work continuously. The
fountains are connected to an elevated water storage tank.
6.4.2 Steam curing of blocks hardened in accordance with 6.3.3 may be
adopted instead of methods speafied in 6.4.1, provided the requirements
of pressure or non-pressure steam curing are fulfilled.
6.5 Drying - After curing the blocks shall be dried for a period of
4 weeks before being used on the work. They shall be stacked with voids
horizontal to facilitate through passage of air. The blocks shall be allowed
to complete their initial shrinkage before they are laid in a wall.
7. SURFACE TEXTURE AND FINISH
7.1 Concrete masonry units can bc given a variety of surface textures
ranging from a very fine close texture to a coarse open texture by the
proper selection, grading, and proportioning of aggregates at the time of
manufacture. Textures may also be developed by treating the face of
the units while still green by wire brushing or combing, by slightly
eroding the surface by playing a fine spray of water upon it, and by
splitting ( split block ). Colour may be introduced by incorporating non-
fading mineral pigments in the facing concrete, or by applying a coloured
cement grout or paint to the face of the units soon after they are removed
from the moulds. Selected coloured aggregates may also be used in the
facing and exposed by washing with water or dilute hydrochloric acid.
7.2 Well made concrete masonry may not require plaster in case of
unimportant buildings in low rainfall areas; two or three coats of a cement
paint being sufficient to render it resistant to rain water. If, however, it
is intended to plaster concrete masonry, the block shall have a sufficiently
rough surface to afford a good key to the plaster. Waterproofing
admixtures may be used for preparing the plaster.
8. PHYSICAL REQUIREMENTS
8.1 General - All units shall be sound and free of cracks or other defects
which interfere with the proper placing of the unit or impair the strength
or performance of the construction. Minor chipping resulting from the
customary methods of handling during delivery, shall not be deemed
grounds for rcjcction.
8.1.1 Where units arc to be used in exposed wall construction, the face
or faces that are to be exposed shall be free of chips, cracks, or other
imperfections, except that if not more than 5 percent of a consignment
contains slight cracks or small chippings not larger than 25 mm, this shall
not be deemed grounds for rkjertion.
8.2 Dimensions -- The overall dimensions of the units when measured
as given in Appendix A shall be in accordance with 3 subject to the
tolerances mentionecl therein.
IS : 2185 ( Part I ) - 1979
8.3 Block Density - The block density, when determined as in
Appendix B, shall conform to the requirements given in 4.
8.4 Compressive Strength - The minimum compressive strength at 28
days being the average of eight units, and the minimum compressive
strength at 28 days of individual units, when tested in the manner
-described in Appendix C, shall be as prescribed in Table 2.
8.5 Water Absorption - The water absorption, being the average of
three u&s, when determined in the manner prescribed in Appendix D,
shall be not more than 10 percent by mass.
Shrinkage - The drying shrinkage of the units when
unrestraine being the average of three units, shall be determined in the
manner described in Appendix E, and shall not exceed 0’1 percent.
8.6 Moisture Movement - The moisture movement of the dried blocks
on immersion ,in water, being the average of three units, when determined
in the manner described in Appendix F, shall not .exceed 0’09 percent.
Hollow ( open and
closed cavity )
Hollow ( open and
closed cavity )
C( 1.5 ) Less than
but not less
than 1 000
Solid load bearing D( 5.0 ) Not less than
units D( 4.0 ) 1 800
TABLE 2 PHYSICAL REQUIREMENTS
( Clauses 4.1,4.2 and-B.4 )
A( 3.5 )
A( 4.5 )
A( 5.5 )
A( 7.0 )
B( 2.0 )
B( 5.0 )
Not less than
but not less
than 1 000
MINIMUM AVERAGE MINIMUM
IS:2185 (Part I)- 1979
9.1 Tests as described in Appendices A to F shall be conducted on
samples of units selected according to the sampling procedure given in 10,
to ensure conformity with the physical requirements laid down in 8.
10.1 The blocks required for carrying out the tests laid down in this
standard shall be taken by one of the methods given in 10.2and 10.3. In
either case, a sample of 20 blocks shall be taken from every consignment
of 5 000 ~blocksor part thereof of the same size and same batch of-manu-
facture. From these samples, the blocks shall be taken at random for
conducting the tests.
10.2 The required number of blocks shall be taken at regular intervals
during the loading of the vehicle or the unloading of the vehicle depend-
ing on whether sample is to be taken before delivery or after delivery.
When this is not practicable, the sample shall be taken from the stack in
which case the required number of blocks shall be taken at random from
across the top of the stacks, the sides accessible and from the interior of
the stacks by opening trenches from the top.
10.3 The sample af blocks shall be marked for future identification of the
consignment it represents. The blocks shall be kept under cover and
protected from extreme conditions of temperature, relative humidity
and wind until they are required for test. The tests shall be undertaken
as soon as practicable after the sample has been taken.
10.4 Number of Tests
10.4.1 .A11 the 20 blocks shall be checked for dimensions and inspected
for visual defects ( See8.1 and 8.2 ).
10.4.2 Out of the 20 blocks, 3 blocks shall be subjected to the test for
block density ( see 8.3 ), 8 blocks to the test for corn
( see 8.4 ), 3 blocks to the test for water absorption P
see 8.5 ) and 3
blocks to the test for drying shrinkage ( see 8.6 ) and later to the test
for moisture movement. The remaining 3 blocks shall be reserved for
retest for drying shrinkage and moisture movement if a need arises.
11. CRITERIA FOR CONFORMITY
11.1 The lot shall be considered as conforming to the requirements of the
specification if the conditions mentioned in 11.2 to 11.5 are satisfied.
11.2 The number of blocks with dimensions outside the tolerance limit
and/or with visual defects, among those inspected shall be nat more than
11.3 For block density and compressive s‘rength, the mean value deter-
mined shall be greater than or equal to the minimum limit specified in
8.3 and 8.4 respectively.
11.4 For drying shrinkage and moisture movement, all the test specimens
shall satisfy the requirements of the test. If one or more specimens
fail to satisfy the requirements, the remaining 3 blocks shall be subjected
to these tests. All these blocks shall satisfy the requirements.
11.5 For water absorption, the mean value determined shall be equal or
less than maximum limit specified in 8.5.
12. MANUFACTURER’S CERTIFICATE
-12.1The manufacturer shall satisfy himself that the masonry units
conform to the requirements of this specification and, if requested, shall
supply a certificate to this effect to the purchaser or his representative.
13. INDEPENDENT. TESTS
13.1 If the purchaser or his representative requires independent tests,
the samples shah be taken before or immediately after delivery, at the
option of the purchaser or his representative and the tests shall be carried
out in accordance with this specification.
13.2 The manufacturers shall supply free of charge the units required for
13.3 Cost of Testing - Unless otherwise specified in the enquiry or
order, the cost of the tests shall be borne as follows:
a) By the manufacturer in the event of the results showing that the
blocks do not conform to this specification, or
b) By the purchaser in the event of the results showing that the
blocks conform to this specification.
14.1 Concrete masonry units manufactured in accordance with this
specification shall be marked permanently with the following information:
a) The identification of the manufacturer;
b) The grade of the unit; and
c) The year of manufacture, if required by the purchaser.
IS : 2185( Part I ) - 1979
14.1.1 Each block may also be marked with._tlie Standard Mark
NOTE - The me of the Standard Mark is governed by the provisions of the
Bureau of Indian Standard5 Act, 1986 and the Rules and Regulations made there-
under. The Standard Mark on products covered by an Indian Standard conveys
the assurance that they have been produced to comply with the requirements of that
standard under a well defined system of inspection, testing and quality control
which is devised and supervised by BlS and operated by the producer. Standard
marked products are also continuously checked by BIS for conformity to that
standard as a further safeguard. Details of conditions under which a Iicence for
the use of the Standard Mark may be granted to manufacturers or producers may
be-obtained frdm the Bureau of Indian Standards.
( Clauses 8.2 and 9.1)
MEASUREMENT OF DIMENSIONS
A-l.1 Overall dimensions shall be measured with a steel scale graduated
in 1 mm divisions. Face shell and web thickness shall be measured with
a caliper rule graduated in 0’5 mm divisions and having parallel jaws
not less than 15 mm nor more than 25 mm in length.
A-2.1 Twenty full size units shall be measured for length, width and
height. Cored units shall also be measured for minimum thickness of
face shells and webs.
NOTE- Thesespecimens shall be used for other tests also.
A-3. MEASUREMENTS AND REPORT
A-3.1 Individual measurements of the dimensions of each unit shall be
read to the nearest diesion of the scale or caliper and the average
A-3.2 Length shall be measured on the longitudinal centre line of each
face, width across the top and bottom bearing surfaces at midlength, and
height on bofh faces at midlength. Face-shell thickness and web thick-
ness shall be measured at the ;hinnest point of each such element 15 mm
IS : 2185( Part I ) - 1979
above, the mortar-bed plane. Where opposite face shells differ in
thickness by less than 3 mm, their measurements shall be averaged. Sash
grooves, dummy joints, and similar details shall be disregarded in the
A-3.3 The report shall show the average length, width, and height of
each specimen, and the minimum face-shell and web thickness and total
web thickness in 200 mm length of walling per course as an average for
the 20 specimens.
( Clauses8.3 and 9.1 )
METHOD FOR THE DETERMINATION OF
B-l.1 Three blocks taken at random from the samples selected in accor-
dance with 10,shall be dried to constant mass in a suitable oven heated
to approximately 100°C. After cooling the blocks to room temperature,
the dimensions of each block shall be measured in centimetres ( to the
nearest millimetre ) and the overall volume computed in cubic centi-
metres. The blocks shall then be weighed in kilograms ( to the nearest
10 g ) and the density of each block calculated as follows:
Mass of block in kg
Volume of specimen in cm*
x 10’ kg/m3
B-l.2 The average for the three blocks shall be taken as the average
( Clauses8.4 and 9.1 )
METHOD FOR THE DETERMINATION OF
C-l.1 Testing Machine -- The testing .machine shall be ~equipped with
two steel bearing blocks ( see Note ) one of which is a spherically seated
block that will transmit load to the upper surface of the masonry speci-
men, and the other a plane rigid block on which the specimen will rest.
When the bearing area of the steel blocks is not sufficient to cover the
bearing area of the masonry specimen, steel bearing plates meeting the
requirements of C-l.2 shall be placed between the bearing blocks and the
capped specimen after the centroid of the masonry bearing surface has
been aligned with the centre of thrust of the bearing blocks ( SGGC-4.1 ).
NOTE- It is desirable that the bearing faces of blocks and lates used for com-
pression testing of concrete masonry have a hardness of not less tL n 60 ( HRC).
C-l.2 Steel Bearing Blocks and Plates - The surfaces of the steel
bearing blocks and plates shall not depart from a plane by more than
0’025 mm in any 15 mm dimension. The centre of the sphere of the
spherically Peated upper bearing block shall coincide with the centre
of its bearing face. If a bearing plate is used, the centre of the sphere of
the spherically seated bearing block shall lie on a line passing vertically
through the centroid of the specimen bearing face. The spherically
seated block shall be held closely in its seat, but shall be free to turn in
any direction. The diameter of the face of the bearing blocks shall be
at least 15 cm. When steel plates are employed between the steel
bearing blocks and the masonry specimen ( see C-4.1 ) the plates shall
have a thickness equal to at least one-third of the distance from the edge
of the bearing block to the most distant corner of the specimen. .In no
case shall the plate thickness be less than 12 mm.
C-2. TEST SPECIMENS
C-2.1 Ei’ght full-size units shall be tested within 72 hours after delivery
to the laboratory, during which time they shall be stored continuously in
normal room air.
C-2.2 Units of unusual size, shape, or strength may be sawed into
segments, some or all of which shall be tested individually in the same
manner as prescribed for full-size units. The strength of the full-size
units shall be considered as ,that which is calculated from the average
measured strength of the segments.
C-2.3 ~For the purpose of acceptance, age of testing the specimens shall
be 28 days. The age shall be reckoned from the time of the addition of
water to the dry ingredients.
C-3: CAPPING TEST SPECIMEN
C-3.0 Bearing surfaces of units shall be capped by one of the methods
described in C-3.1 and C-3.2.
C-3.1 Sulphur and Granular Mat&als - Proprietary or laboratory
prepared mixtures of 40 to 60 percent sulphur ( by mass ), the remainder
being ground fire clay or other suitable inert material passing 150-micron
IS sieve with or without a plasticizer, shall be spread evenly on a non-
absorbent surface that has been lightly coated with oil ( see Note ). The
sulphur mixture shall be heated in a thermostatically controlled heating
pot to a temperature suficient to maintain fluidity for a reasonable period
of time after contact with. the capping surface. Care shall be exercised
to prevent overheating, and the liquid shall be stirred in the pot just
before use. The capping surface shall be plane within 0’075 mm in 40 cm
and shall be sufficiently rigid and so supported as not to be measur-
ably deflected during the capping operation. Four 25 mm square steel
bars shall be placed on the surface plate to form a rectacgular mould
approximately I2 mm greater in either inside dimension than the masonry
unit. The mould shall be fillcd~to a depth of 6 mm with molten sulphur
material. The surface of the unit to be capped shall quickly be brought
into contact with the liquid, and the specimen, held so that its axis is at
right angles to the surface of the capping liquid, shall be inserted. The
unit shall be allowed to remain undisturbed until solidification is com-
plete. The caps shall be allowed to cool for a minimum of 2 hodrs
before the specimens arc tested. Patching of caps shall not be permitted.
Imperfect caps shall he removed and replaced with new ones.
NOTE- The USCof oil on capping p1atc.s may be onlittv~l if it is found that plate
and unit cm br separated without damaging the cap.
C-3.2 Gypsum Plaster Capping -- A~neat paste of‘spccial high-strength
plaster ( see Note under C-4.1 ) and water shall be spread evenly on a
non-absclrbent surface that has been lightly cc!atcd with oil. Such
gypsum plaster, when gauged with water at thr capping cousistcncy,
shall have a compressive strength at a 2-hour age of not less than
25 N/mm2, when tested as 50 mm cubes. The casting surface p!ate shall
conform to the requirements described in C-3.1. The surface of the unit
to be capped shall be brought into contact with the capping paste; the
specimen which is held with its axis at right angles to the capping surface,
shall be firmly pressed down with a single motion. The avcragc thick-
ness of the cap shall be not more than 3 mm. Patching of caps shall not
be permitted. Imperfect caps shall be removed and replaced with new
ones. The caps shall be aged for at least 2 hours before the specimens are
C-4.1 Position of Specimens -- Specimens shall be tested with the
centroid of their bearing surfaces aligned vertically with the ccntre of
thrust of the spherically. seated steel bearing block of the testing machine
IS f 2185 ( Part I ) - 1979
( seeNote ). Except for special, units’ intended for use with their cores
in a horizontal direction, all hollow concrete masonry units shall be tested
with their cores in a vertical direction. Masonry units that are 100
percent solid and special hollow units intended for use with their hollow
cores in a horizontal direction may be tested in the same direction as in
NOTE - For homogeneous materials, the centroid of the bearing surface shall be
considered to be vertically above the centre of gravity of the masonry unit.
C-4.2 Speed of Testing - The load up to one-half of the ‘expected
maximum load may be applied at any convenient rate, after which the
control of the machine shall be adjusted as required to give a uniform
rate of travel of the moving head such that the remaining load is applied
in not less thsn one nor more than two minutes.
C-5. CALCULATION AND REPORT
C-5.1 The compressive strength of a concrete masonry unit shall be taken
as the maximum load in Newtons divided by the gross cross-sectional area
of’ the unit in square millimetres. The gross area of a unit is the total
area of a section perpendicular to the direction of the load, including
areas within cells and within re-entrant spaces unless these spaces are to
be occupied in the masonry by portions of adjacent masonry.
C-5.2 Report the results to the nearest 0’1 N/mms separately for each
unit and as the average for the 8 units.
( Clauses 8.5 and 9.1 )
METHOD FOR THE DETERMINATION OF ABSORPTION
D-l.1 The balance used shall be sensitive to within 0’5 percent of the
mass of the smallest specimen tested.
D-L.2 Three full-size units shall be used.
D-2.1 Saturation - The test specimens shall be completely immersed
in water at room temperature for 24 hours. The specimens shall then be
weighed, while suspended by a metal wire and completely submerged in
water. They shall be removed from the water and allowed to drain
for one minute by placing them on a 10 mm or coarser wire mesh,
visible surface water being. removed with a damp cloth, and immediately
D-2.2 Drying - Subsequent to saturation, all specimens shall be dried
in a ventilated oven at 100 to 115°C for not less than 24 hours and until
two successive weighings at intervals of 2 hours ,show an increment of
loss not greater than 0’2 percent of the last previously determined mass
of the specimen.
D-3. CALCULATION AND REPORT
D-3.1 Absorption - Calculate the absorption as follows:
Absorption, kg/m5 = A _ c; x 1 000
Absorption, percent ‘= 7 x 100
A = wet mass of unit in kg,
B = dry mass of unit in kg, and
C - suspended immersed mass of unit in kg.
D-3.2 Report - Report all results separately for each unit and’as the
average for the three units.
( CZuuses8.6 and 9.1)
METHOD FOR THE DETERMINATION OF
E-l. NUMBER OF TESTS
E-l.1 Of the samples selected in accordance with 10, three shall be tested
for drying shrinkage. Three more blocks shall be set aside and stored
in air-tight containers at normal room temperature so as to be available
*for duplicate tests if they are required at a later stage ( see Note ).
NOTE - In order to facilitate storage, instead of blocks, sections cut from these
additional blocks may be stored until necessary in separate air-tight containers at
normal room temperature.
IS t 2185 ( Part I ) - 1979
E-2.1 Measuring Apparatus - A measuring apparatus shall be used
which incorporates a micrometre gauge or a suitable dial gauge reading
accurately to 0’002 5 mm. This gauge shall be rigidly mounted in a
measuring frame and have a recessed end which may be located upon a
5-mm diameter ball or other reference point cemented on the specimen.
The other end of the frame shall have a similar recessed seating which
may be located upon the other ball or reference point in the specimen.
An Invar steel rod of ‘suitable length with 5-mm diameter hemispherical
ends or with 5-mm iliameter steel balls mounted on the ends, shall be
used as a standard of length against which readings of the gauge may be
checked, thus enabling corrections to be made for any change in the
dimensions of the apparatus between successive measurements of a test
specimen. The apparatus shall preferably be adjusted for specimens of
different lengths and Invar rod of lengths near to those of the specimens
to be tested shall be available.
E~2.2 Drying Oven - The drying oven shall comply with the following
a) It shall have an internal volume equivalent to not less than
8 litres per specimen, with a minimum total volume of 50 litres.
b) It shall be reasonably air-tight and shall be provided with a fan
to keep the air circulating effectively during the drying of the
c) It shall be capable of maintaining a constant temperature of
50 f 1°C.
d) The relative humidity ofthe air in the oven shall be controlled
at approximately 17 percent by means of saturated calcium
chloride solution. Suitable dishes or trays containing this solu-
tion shall be
rovided to give an exposed area of solution not
less than 10 cm for each litre of volume of the oven. The dishes
or trays shall contain sufficient solid calcium chloride to show
above the surface of the solution throughout the test. .
E-3. PREPARATION OF SPECIMENS
E3.1 One sample shall be cut from each of the blocks such that the
length of each specimen is not less than 15 cm and the cross section is as
near to 7’5 X 7’5 cm as practicable in the case of solid blocks and
7’5 cm X thickness of the wall in the case of other blocks. Two reference
points consisting of 5 mm diameter steel balls or other suitable reference
points providing a hemispherical bearing shall be cemented with neat
rapid-hardening Portland cement or other suitable cementing material
at the centre of each end of each specimen after drilling or cutting a
shallow depression. After fixing, the surface of the steel balls shall.be
wiped clean. of cement, and dried and coated with lubricating grease to
prevent corrosion. The specimens shall then be completely immersed in
water for 4 days, the temperature being maintained at 27 f 2°C at least
for the last 4 hours.
E-4. PROCEDURE FOR TESTING
E-4.1 Immediately after removal of the specimens from the water, the
grease shall be wiped from the steel balls and the length of each specimen
measured to an accuracy of 0’002 5 mm by the apparatus described
in D-2.1. This shall be taken as the original wet measurement.
NOTE- The instrument reading required is not the absolute length of the speci-
men but the difference in length between the specimens and an Invar rod of
E-4.2 The specimens shall then be dried for at least 44 hours in an oven
of the type described in E-2.2, at the specified temperature and humidity.
The specimens shall then be removed from the oven and cooled for at
least 4 hours in a desiccator .containing solid calcium chloride or a
saturated solution of calcium chloride. Each specimen shall then be
measured as described in E-4.1, at a temperature of 27 f 2°C.
E-4.3 The cycle of drying, cooling and measuring shall be repeated until
constant length is attained, that is when the difference between conse-
cutive readings separated by a period of drying of at least 44 hours
followed by cooling for at least 4 hours, is less than 0’005 mm for a
15 cm specimen and pro ruta for a larger specimen. The final reading
shall be taken as the dry measurement.
E-4.4 During the above drying process further wet specimen shall not be
placed~in the same oven and there shall be free access of air to all surfaces
of the specimen.
E4.5 After the dry measurement has been taken, the length ~ofthe
specimen shall be measured, adjacent to the steel balls, to the nearest
mrllimetre and this shall be taken as the ‘dry length’.
E-5. CALCULATION OF RESULTS
E-5.1 The ‘drying shrinkage’ shall be calculated for each specimen as the
difference between the ‘original wet measurement’ and the ‘dry measure-
ment’ expressed as a percentage of the ‘dry length’.
E-5.2 Report all results separately for each unit.
IS 3 2185m(Part I ) - 1979
( Clauses 8.7 and 9.1 )
METHOD FOR THE DETERMINATION OF
F-l.1 The specimens which have previously been used for the drying
shrinkage test ( see Appendix E ) shall after the completion of~that test,
be immersed in water for 4 days, the temperature being maintained at
27 f 2°C for at least 4 hours prior to the removal of the specimens and
the wet length measured. The moisture movement shall be determined
as the difference betiveen the dry and wet lengths and expressed as a
percentage of the dry length for each specimen.
F-l.2 Should the value obtained with any one of the three specimens
tested be greater than the limit specified in 8.7, the test shall be repeated
on the further three blocks which -were set aside. In repeating the
moisture movement test, the drying shrinkage test shall be repeated if
the previous specimens have failed on that test also; otherwise, the drying
shrinkage test may be omitted. The three new specimens, in that event,
shall be dried to constant length at 50 f 1°C measured after cooling and
the moisture movement test-carried out as described in F-1.1.
IS : 2185( Part I ) - 1979
( Continuedfrom fiage 2 )
Precast Concrete Products Subcomniittee, BDC 2 : 9
DEPUTY DIRECTOR, STANDARDS Research, Designs 8t Standards Organization
(B&S) ( Ministry of Railways )
STANDARDS~(B&S )-II ( Ahnat )
DEVELOPMENTMANAQE~ Hindustan Prefab Ltd, New Delhi
DIRECTOR ( CSMRS ) Central Water Commission, New Delhi
DEPUTY DIRECTOR (-CSMRS )
( Ahnat )
SRRI V. G. GOKHALE
SHRI B. K. JINDAL
Bombay Chemicals Pvt Ltd, Bombay
Central Building Research Institute ( CSIR ),
Da S. S. REESI ( Aftanatc )
SHRI L. c, LA1
DR A. K. MULLICK,
In Personal Capacity ( B/17 West End, New Delhi )
Clement Research Institute of India, New Delhi
DR S. C. MAITI ( Altcmats )
SH~I S. NAHAROY Engineering Const&ction Corporation Ltd,
SHRI A. RAMAKRISHNA ( &?mats )
SHRI D. B. NAIK Engineer-in-Chief’s Branch, Army Headquarters
SHRI 0. P. BHATIA ( Ahnat )
.SHRI K. K. NAMBEAR
SHRI P. S. NATARAJAN
Da A. V. R. RAO
SHRI G. T. BEIDE ( &?mats )
SRRI V. RAMALINOAM
SHRI B. G. SHIRKE
SHRI R. T. PAWAR ( Ahmat )
SHRI C. N. SRINIVASAN
SHRI C. N. RAQHAVENDRAN
SHRI B. T. UNWALLA
SHRI E. T. ANTIA ( Alternate )
DR B. VENKATEBWARLU
In Personal Capacity ( ‘Ramana&rya’ 11 First
Crescent Park Road, Gandhinagar, Adyar,
Tamilnadu Housing Board, Madras
National Buildings Organization, New Delhi
Neyveli Lignite Corporation Ltd, Neyveli
B. G. Shirke & Co, Pune
M/s C. R. Narayana Rao, Madras
The Concrete Association of India, Bombay
Struc;oTrLlengineering Research Centre ( CSIR ),
BUREAU OF IND4AN STANDARDS
Manak Bhavan, 9 Bahadur Shah Zafar Marg, NEW DELHI 110002
Telephones: 331 01 31, 331 13 75 Telegrams: -Manaksanstha
( Common to all Offices)
Regional Offices: Telephone
Central : Manak Bhavan, 9 Bahadur Shah Zafar Marg,
331 01 31
NEW DELHI 110002 331 1375
*Eastern : 1/14 C. I. T. Scheme VII M, V. I. P. Road, 36 24 99
Maniktola. CALCUTTA 700054
Northern : SC0 445-446, Sector 35-C,
2 18 43
CHANDIGARH 160036 3 16 41
41 24 42
Southern : C. -I. T. Campus, MADRAS 600113 41 25 19
twestern : Manakalaya, E9 MIDC, Marol, Andheri ( East ), 6 32 92 95
‘Pushpak’. Nurmohamed Shaikh Marg, Khanpur,
2 63 48
AHMADABAD 380001 2 63 49
$Peenya lndust rial Area 1st Stage,. Bangalore Tumkur Road 38 49 55
38 49 56
Gangotri Complex, 5th Floor. Bhadbhada Road, T. T. Nagar, 667 16
Plot No. 82/83. Lewis Road. BHUBANESHWAR 751002 5 36 27
53/5. Ward No. 29, R.G. Barua Road, 5th Byelane, 3 31 77
5-8-56C L. N. Gupta Marg ( Nampally Station Road ), 23 1083
R14 Yudhister Marg, C Scheme, JAIPUR 302005
6 34 71
6 98 32
117/418 B Sarvodaya Nagar, KANPUR 208005
21 68 76
21 82 92
Patliputra Industrial Estate, PATNA 800013 6 23 05
T.C. No. 14/1421.University P.O.. Palayam 16 21 04
TRIVANDRUM 695035 16 21 17
Inspection Offices ( With Sale Point ):
Pushpanjali, First Floor, 205-A West High Court Road, 2 51 71
Shankar Nagar Square, NAGPUR 440010
Institution of Engineers ( India ) Building, 1332 Shivaji Nagar, 5 24 35
*Sales Officein Calcuttais a( S ChowringherApproach,P. 0. ~Princep27 68 00
tSsler Office in Bombay I8 at Novrltv Chambers, Grant Ro&d, 89 85 28
#Sales Office in Bangalore is at Unity Building, Narasimharrja Square, 22 38 71
Reprography Unit, BIS, New Delhi, India
AMENDMENT NO. 1 MAY 1984
IS:2185(Part l)-1979 SPECIFICATION FOR CONCRETE
PART 1 HOLLOW AND SOLID CONCRETE BLOCKS
(Page 14, clause 11.3) - Substitute the following
for the existtng clause:
'11.3 For block density (see Note in Table ~2) and
compressive strength, the mean value determined shall
be greater than or equal to the minimum limit specified
in 8.3 and 8.4 respectively.'
(Page 12, TabZe 2) - Add the following note in
the table at the end:
'Note - The density of block is specified for
the guidance of manufacturers; while ordering the
blocks, purchaser shall specify the grade only.'
Reprograpt~y Unit, BIS, New Delhi, India